Polyimide-based aerogel foams, via emulsion-templatingPolymer
Nicholas Teo, Zipeng Gu, Sadhan C. Jana∗
Department of Polymer Engineering, The University of Akron, 250 South Forge Street, Akron, OH, 44325-0301, USA
H I G H L I G H T S
• Oil-in-oil emulsion templating produces aerogel foams from polyimides.
• PEO-PPO-PEO block copolymer surfactant stabilizes oil-in-oil emulsions.
• Surfactant reduces macrovoid size but increases polyimide strand size.
• Surfactant organizes to produce higher contact angle and promotes oil absorption.
A R T I C L E I N F O
Keywords: Aerogels Aerogel foams Polyimide Oil-in-oil emulsions Emulsion-templating
A B S T R A C T
An oil-in-oil emulsion-templating method is used to fabricate polyimide aerogel foam materials. These materials contain micrometer size voids (macrovoids) in conjunction with inherently produced meso- and macropores in polyimide gels. Polyamic acid is first synthesized from diamines and dianhydrides and then chemically imidized to obtain a sol. An immiscible oil-type dispersed phase is introduced in the sol via emulsification and the sol is subsequently allowed to transition into a gel, thereby locking the dispersed phase droplets within the structure. The gel is subsequently dried under supercritical conditions to obtain aerogel foams. This paper evaluates the stability of the oil-in-oil emulsion used for templating with reference to the gel times of the continuous phase. Specifically, the effects of surfactant concentration on macrovoid size, mesopore size, and mechanical properties of the aerogel foams are investigated. In addition, water and oil absorption behavior of the aerogel foams are studied.
Polyimides were first reported in 1908, although its usage increased after the late 1950s once high molecular weight polyimides were suc- cessfully prepared . These materials possess excellent properties such as high thermal, hydrolytic, and radiation stability, as well as good mechanical strength and electrical properties at elevated temperatures [2,3]. These properties, in conjunction with its gel forming capability, have qualified polyimides as an appropriate candidate for aerogel fabrication. Polyimide aerogels and their hybrids have been reported in literature . For example, the network structure of silica aerogels were coated with a layer of polyimide to impart structural integrity and improve load bearing capabilities . The step-growth nature of polyimide synthesis also accommodates a variety of monomers for tailoring the mechanical properties, shrinkage, and surface energy of polyimide aerogels [6,7]. Traditionally, polyimides are fabricated using the Dupont two-step process. First, polyamic acids are obtained by re- acting dianhydrides and diamines. The second step involves chemical
imidization using acetic anhydride as a dehydrating agent and pyridine as a catalyst, whereby the amic acid functional group is converted to the imide functional group . Other synthesis routes for polyimide aerogels have also been reported, such as ring opening polymerization  and substituting isocyanates for amines .
Aerogels are frequently fabricated in a cylindrical monolith shape, although recent studies have reported both flexible films and micro- particle forms [11,12]. The high thermal stability and the close proxi- mity of aerogel pore sizes to the mean free path of air molecules impart excellent thermal insulation properties in polyimide aerogels. This has seen polyimide aerogels deployed as insulation for entry/re-entry ve- hicles and extravehicular activity suits . The inherent low dielectric properties of polyimide aerogels also make them suitable for fabrication of antenna [14,15] and membrane separators for batteries . In addition, the open pore structures of polyimide aerogels, with both meso- (dia 2–50 nm) and macropores (dia> 50 nm), have shown to be useful in filtering airborne nanoparticles. These aerogels have been shown to achieve a high separation efficiency of 99.99%, while
https://doi.org/10.1016/j.polymer.2018.10.030 Received 30 July 2018; Received in revised form 8 October 2018; Accepted 15 October 2018
∗ Corresponding author. E-mail address: [email protected]
Polymer 157 (2018) 95–102
Available online 16 October 2018 0032-3861/ © 2018 Elsevier Ltd. All rights reserved.
tion vs. filtration efficiency and macropore fraction vs. air permeability relationships. This study's takeaway was that high air permeability and high filtration efficiency require high fractions of macropores and me- sopores respectively. However, aerogel monoliths prepared by the methods reported in literature do not allow independent control of both meso- and macropore fractions. This necessitated another method of incorporating macropore fractions in aerogel materials without altering the mesopore content, bearing in mind that the final structures should be one-component, free-standing, and hierarchical. This served as the motivation for the development of aerogel foams, fabricated via in- clusion of micrometer sized voids, defined as macrovoids, into in- herently porous aerogel structures. The macrovoids allow quick transfer of fluids through the aerogel structures, thus allowing higher fluid permeability.
Aerogel foams have previously been fabricated using a number of methods. Gu and Jana  had used a solid template of co-continuous polymer systems to synthesize polyurea aerogel foams. Wang and Jana  used a solution of polyethylene oxide to obtain micrometer size voids in syndiotactic polystyrene (sPS) aerogels. Recently, Teo and Jana  successfully used a water-in-oil emulsion-templating method to introduce spherical, ∼20 μm sized macrovoids in macroporous sPS aerogel structures. In this work , sPS and a nonionic surfactant were first dissolved in toluene at high temperature and the solution was emulsified using deionized water. The sPS solution turned into a gel when cooled to room temperature, thus locking in the emulsified water droplets within the vitrified structure. The gel was supercritically dried to yield sPS aerogel foam materials. However, this water-in-oil emul- sion templating method cannot be extended to water-sensitive mono- mers such as those encountered in polyimide systems. On the other hand, aerogel foams produced from high temperature polyimides have the potential for expanded applications such as in hot air filtration. In view of this, the present work details an oil-in-oil (O/O) emulsion- templating method for incorporation of significant fractions of macro- voids in polyimide aerogel structures. This yields polyimide aerogel foams with macrovoids (∼30 μm) seen in foams, as well as mesopores found inherently in polyimide aerogels.
2. Experimental section
Pyromellitic dianhydride (PMDA) was purchased from Alfa-Aesar (Haverhill, MA) and 2,2′-dimethylbenzidine (DMBZ) was purchased from Shanghai Worldyang Chemical Co. Ltd (Shanghai, China). Tris(2- aminoethyl)amine (TREN) and surfactant F127® (trademark of BASF) were purchased from Sigma Aldrich (Milwaukee, WI). Pyridine, acetic anhydride, cyclohexane, and acetone were purchased from Fisher Scientific (Ontario, NY). N,N-dimethylformamide (DMF) was purchased from VWR International (Radnor, PA) and n-heptane was purchased from EMD Millipore (Billerica, MA).
2.2. Fabrication of aerogel foams
An O/O emulsion-templating method was used in this work to ob- tain micrometer size oil droplets dispersed in the sol. The sol transi- tioned into a gel, thus locking the emulsified oil droplets within the gel structures. This process resembles the fabrication of polyHIPEs [21–23], with the exception that the continuous oil-phase in this study was initially an organic sol, which later turned into a gel with its in- herent pores filled by the organic solvent.
All materials were stored in desiccators and used as purchased, with the exception of F127® surfactant, which was dried in a vacuum oven for at least 30min at a temperature of 35 °C prior to dissolution to mitigate the effect of absorbed moisture. The continuous oil phase was
first prepared by dissolving PMDA and F127® surfactant in DMF over a period of at least 30min, to ensure full dissolution of the surfactant. DMBZ was dissolved in DMF, added to the PMDA and surfactant solu- tion, and magnetically stirred for 2min at 1600 rpm to form the polyamic acid solution. TREN, acetic anhydride, and pyridine were added at the same time together to the polyamic acid solution to serve respectively as the crosslinker, dehydrating agent, and catalyst. These three reagents had to be added all at once as the fast reaction kinetics of the crosslinker (TREN) would lead to immediate precipitation of the crosslinked materials if added separately. The reaction was conducted at room temperature of 19 °C in a sealed glass vial under air, with the reaction scheme shown in Fig. 1. The final reaction mixture was stirred magnetically for 3min followed by addition of the dispersed phase (cyclohexane or n-heptane) and stirred for an additional 5min. This allowed for the viscosity of the solution to increase with conversion, imparting increased stability to the O/O emulsion. For neat polyimide samples without any surfactant or dispersed phase, this step involved further stirring of only 1.5min, to allow transfer to the molds before gelation. A typical sample with 30 vol% dispersed phase and 0.5 vol% surfactant based on the continuous phase was prepared from 0.114 g PMDA, 0.017 g F127®, 0.106 g DMBZ, 0.015 g TREN, 0.360 g acetic anhydride, 0.307 g pyridine, 2.5mL DMF, and 1.67mL dispersed phase (cyclohexane or n-heptane). The above recipe produced a polymer concentration of 7.4 wt% in the solution.
The final mixture was poured into cylindrical molds and allowed to gel. The selection of monomers, crosslinker content, and overall polymer concentration in the sol allowed fast gelation and vitrification of the emulsion while facilitating pouring of the sol in the mold. The gels were aged in the molds for 48 h before demolding. The presence of surfactant delayed gelation of the system. Accordingly, the gels were left in the molds for 48 h to ensure completion of crosslinking and imidization reactions. The demolded gels were solvent exchanged se- quentially with 25 vol% acetone/75 vol% DMF, 50 vol% acetone/50 vol % DMF, 25 vol% acetone/75 vol% DMF, and finally with 100 vol% acetone at 12-h intervals. In addition, the gels were further washed with 100 vol% acetone for an additional 5 times at 12-h intervals to remove as much of the DMF as possible. The gels were subsequently solvent exchanged with liquid carbon dioxide in an autoclave by washing with 100 vol% liquid carbon dioxide for 6 times at 1.5 h intervals. The liquid carbon dioxide infused gels were subsequently dried under supercritical condition of carbon dioxide at 50 °C and 11MPa. The surfactant
Fig. 1. Reaction scheme for synthesis of polyimide.
N. Teo et al. Polymer 157 (2018) 95–102
concentration was varied between 0.5 vol% and 5 vol% to impart sta- bility of the O/O emulsion against creaming and coalescence before gelation of the continuous phase.
As reference materials, polyimide aerogels were also synthesized with surfactant without dispersed phase, and without surfactant and without dispersed phase (neat PI).
2.3. Characterization of oil-in-oil (O/O) emulsions
Interfacial Tension Measurement. The interfacial tension between the dispersed (cyclohexane or n-heptane) and the continuous (DMF) phases was measured using a Du Noy tensiometer (Interfacial Tensiometer 70545, Central Scientific Co., VA). First, the surfactant was dissolved in DMF at concentrations of 0.5, 2.5, and 5.0 vol%. Next, 20mL of the dispersed phase was gently added to the top of the surfactant solution in DMF by pouring the liquid over a clean glass slide to prevent emulsi- fication and droplet formation during pouring. Interfacial tension was then recorded in triplicate by placing the Du Noy ring at the interface of these two phases.
Emulsion Droplet Size. The droplet size distribution of O/O emulsions (prepared by mixing surfactant, DMF, and cyclohexane/n-heptane) was studied using Olympus BX51 optical microscope (Center Valley, PA). For this purpose, a drop of emulsion was placed on a microscope slide with a depression and its optical images were recorded. The images were analyzed using ImageJ software to yield droplet size distributions from the diameter data of more than 100 droplets.
2.4. Characterization of aerogel foams
Aerogel Foam Morphology and Macrovoid Size Distribution. The mor- phology of aerogel foams was obtained using a scanning electron mi- croscope (JSM5310, JEOL, MA). An accelerating voltage of 5 kV and emission current of 20mA was used to capture the SEM images. For this purpose, a representative piece of fractured aerogel foam specimen was mounted on an aluminum stub using carbon tape, followed by sputter coating with silver (ISI-5400 Sputter Coater, Polaron, UK). The mac- rovoid size distribution was obtained from the analysis of SEM images using ImageJ software. For each specimen, more than 100 macrovoids were considered for determining the macrovoid size distribution. The size of polyimide strands in SEM images was measured using ImageJ software.
IR: Infrared spectra was recorded on a Nicolet iS50 FTIR tri-detector spectrophotometer (Thermo Scientific, MA).
TGA: Thermogravimetric analysis was conducted under N2 with a Q50 thermogravimetric analyzer (TA Instruments, DE) using a heating rate of 20 °C/min, up to 800 °C.
Porosity and Pore Volume: Porosity was calculated from the values of skeletal (ρs) and bulk density (ρb) using equation (1). The values of skeletal density were obtained using a helium pycnometer (AccuPyc II 1340, Micromeritics Instrument Corp., GA). Bulk density of the aerogel foams was calculated from the values of mass and volume of the foam specimens.
= − ×porosity ρ ρ
(1 ) 100%b
Total pore volume (Vtot) was calculated from the bulk and skeletal density according to equation (2):
= −V ρ ρ 1 1
tot b s (2)
Shrinkage: The diameter (d0) of cylindrical plastic molds for poly- imide gels was 13mm. The diameter shrinkage was calculated from the values of diameter (d) of dried aerogel and d0.
BET surface area: Brunauer-Emmett-Teller (BET) surface area of the aerogels and aerogel foams were obtained from N2 adsorption-deso- rption isotherms at 77 K using a Micromeritics Tristar II 3020 analyzer
(Micromeritics Instrument Corp. GA). Gel times and Viscosity: The gel time of the polyimide solution at
room temperature was obtained from the crossover point of the storage (G') and loss (G'') moduli measured using an ARES G2 Rheometer (TA Instruments, New Castle, DE). For this purpose, the final reaction mixture was poured into a solvent trap and loaded into the rheometer fitted with a 50mm cone and plate set up. The rheometer was operated at a constant angular frequency of 1 rad/s at 10% strain.
Compressive Modulus: Compressive modulus of aerogel and aerogel foam specimens were obtained as per ASTM D695-15 method from compressive tests using an Instron 5567 tensometer (Norwood, MA) fitted with a 1 kN load cell and a compression rate of 1.3mm/min. Aerogel and aerogel foam specimens were molded into cylindrical shapes with height to diameter ratio of 2:1. The final aerogel specimens were grinded to ensure smooth and parallel surfaces. The compressive modulus value was obtained from the slope of stress vs. strain curves at low strain, typically ∼0.01mm/mm.
Contact Angle: The values of contact angle of deionized water were measured using a Rame-hart Model 590 Advanced Automated Goniometer/Tensiometer using the DROPimage Advanced software (Succasunna, NJ). For this purpose, aerogel specimens were first com- pressed to remove all the pores before placing water drops on them.
3. Results and discussion
3.1. Emulsion formation
The O/O emulsions prepared from the surfactant and the continuous and dispersed phase liquids were examined to obtain a first approx- imation of the dispersed phase droplet size distribution in such systems. This was done without any polyimide precursor monomers in the system. Both DMF/cyclohexane and DMF/n-heptane systems exhibited intrinsically low interfacial tension values, respectively at 3.6 and 4.0 mN/m (Table 1). The interfacial tension values reduced to 2.0 and 3.5 mN/m respectively for DMF/cyclohexane and DMF/n-heptane sys- tems with the addition of F127® surfactant. The surfactant concentra- tion above 0.01 vol% had no additional effect on interfacial tension, indicating that surfactant concentrations 0.5, 2.5, and 5.0 vol% were above the critical micelle concentration (CMC). This is in line with other CMC studies of Pluronic® block copolymers in aqueous systems .
A continuous phase of the emulsion system was also prepared by mixing DMF, acetic anhydride, pyridine, and F127® in the same pro- portion as were used later in polyimide gel fabrication. The droplet size distributions for such a system are presented in Fig. 2 as function of surfactant concentration. The values of maximum, minimum, and mean droplet size are listed in Table 2.
Several trends became apparent from the data presented in Fig. 2. The dispersed phase droplets were generally smaller in the case of
Table 1 Interfacial tension of DMF/cyclohexane/F127® and DMF/n-heptane/F127®
Interfacial tension (mN/m)
DMF cyclohexane 0 3.6 ± 0.1 0.01 2.0 ± 0.0 0.5 2.0 ± 0.0 2.5 2.0 ± 0.1 5.0 2.0 ± 0.1
n-heptane 0 4.0 ± 0.0 0.01 3.5 ± 0.0 0.5 3.5 ± 0.1 2.5 3.4 ± 0.1 5.0 3.4 ± 0.1
N. Teo et al. Polymer 157 (2018) 95–102
cyclohexane. It is noted from the data in Table 2 that the maximum droplet diameter for cyclohexane with 0.5 and 2.5 vol% surfactant concentration were 191.9 and 77.1 μm respectively, while the corre- sponding maximum droplet diameter for the n-heptane system was 267.6 and 141.2 μm respectively. Such a difference in size can be at- tributed to lower values of interfacial tension in the case of DMF/cy- clohexane system, as listed in Table 1. It is intuitive that higher sur- factant concentration also led to stabilization of larger interfacial area between the polar and the non-polar phases, resulting in smaller dis- persed phase droplets. The mean droplet diameter in the case of DMF/ cyclohexane system were 61.7 ± 34.5 μm, 50.2 ± 33.5 μm, and 33.5 ± 13.0 μm respectively for surfactant concentration of 0.5, 2.5, and 5 vol%. A similar trend, i.e., the mean droplet size reduced with an increase of surfactant concentration, is apparent in the case of DMF/n- heptane system.
It is recognized that O/O emulsions have poor stability due to weaker associations of the traditional surfactants at the O/O interface and higher mutual solubility between the dispersed and continuous phases . These inherent characteristics lead to rapid flocculation, coagulation, and ultimately phase separation in O/O emulsion systems, with more significant Ostwald ripening than in aqueous emulsions . This was prevalent in the experimental system considered in this work, as presented in Fig. 3 for the DMF/n-heptane/F127® emulsion with 5 vol% surfactant concentration. The images in Fig. 3 show significant coalescence of the dispersed phase droplets in just 6 s after the emulsion was placed on the optical microscope stage.
The presence of surfactants also increased the viscosity of the con- tinuous phase. Teo and Jana  observed an increase of viscosity in solution of F127® surfactant in DMF, e.g., the viscosity increased from 0.87mPa-s for DMF to 2.3mPa-s with 5 vol% F127® in solution. Such an increase in viscosity has potential impacts on the diffusion kinetics and the gel time of the polyimide system. The presence of polyimide pre- cursor materials also increases the viscosity of the continuous phase. The higher viscosity of the continuous phase can affect the size of the
dispersed phase droplets in the emulsion and the macrovoids in the gel structures. In view of the above, the morphology of aerogel foam structures is discussed next.
3.2. Morphology of aerogel foam
The aerogel foams primarily consist of macrovoids (as in foams) in a porous polymer domains (as in aerogels). The porous polymer domains in turn are formed by the networks of polymer strands with embedded inherent pore structures. The macrovoids presented in Fig. 4 originated from the dispersed phase liquid droplets in the starting O/O emulsions. Recall that the dispersed phase liquid was replaced by acetone in the solvent exchange step and finally by liquid carbon dioxide in the su- percritical drying step. The images presented in Fig. 4 confirm that the macrovoids produced in polyimide aerogel foams had a certain un- iqueness. They were not connected by open pores as in polyHIPEs  or in emulsion-templated syndiotactic polystyrene (sPS) aerogel foams . However, this type of aerogel foams cannot be strictly classified as closed cell foams as the domains that separate the macrovoids are mesoporous in nature (Fig. 4g). A closer look at Fig. 4g reveals that polyimide strands organized more densely at the macrovoid surface layers than in the bulk. As…